- Lost-foam casting
Lost foam casting (LFC) is a type of
investment castingprocess that uses foampatterns as the investment. This method takes advantage of the properties of foam to simply and cheaply form castings that would be difficult or impossible, using normal " cope and drag" techniques.
Lost foam casting Process
Polystyrenepattern is either carved or molded.
Polystyrene may be carved with traditional carving tools or hot-wire cutting tools. It is also easily sanded.
Injecting Polystyrene in a Mold
Polystyrene, which contains pentaneas a blowing agent, is commonly used for beads. The beads are first pre-expanded and then stabilized, after which, they are blown into a moldto form pattern sections. A steam cycle then causes them to expand fully and fuse together, following which, it undergoes an in-mold cooling cycle. If the final shape is too complex for a single mold, it is molded in sections. The shaped foam sections are aged, and then glued together to form a cluster.
Preparing Final Investment for Casting
Risers and gates are also likewise attached to the pattern. (They must be part of the casting to minimize shrinkage.) Next, the foam cluster is coated with ceramic investment, either by dipping, spraying or pouring. The coating forms a barrier so that molten metal does not penetrate or cause sand erosion during pouring. Coating also helps to protect the structural integrity of the casting.
After the coating dries, the cluster is placed into a flask and backed up with un-bonded sand. Mold compaction is then performed, using a vibration table to ensure uniform and proper compaction. Once compacted, the mold is ready to be poured.
Automatic pouring is commonly used in LFC, as the pouring process is significantly more critical than in conventional
foundrypractice. With LFC process, cleaning is easier and requires fewer operations, since there are no fins or parting lines to remove.
LFC originated on
April 15, 1958, when H.F. Shroyer patented the use of foam patterns, imbedded in traditional green sand, for metal casting(U.S. patent 2830343). In his patent, a pattern was machined from a block of expanded polystyrene (EPS), and supported by bonded sand during pouring. This process is now known as the " full mold process".
The polystyrene foam pattern left in the sand is filled by the molten metal, precisely duplicating all of the features of the pattern. Like the
lost waxprocess, a pattern must be produced for every casting made.
With the full mold process, the pattern is usually machined from an EPS block and is used to make a one-of-a kind casting. The "full mold process" was originally known as the "
lost foam process".
1964, M.C. Flemmings used unbonded sandfor the process. Flemming’s method is today known as "lost foam casting" (LFC). LFC is differentiated from full mold by the use of unbonded sand, as opposed to bonded sand that is used in the full mold process. Currently, more foundries in North Americause the LFC process than the full mold process.
Foam casting techniques (both “full mold” and LFC) have been referred to by a variety of generic and proprietary names. Among these are “full mold”, “cavityless casting”, “lost foam”, “evaporative foam casting”, “evaporative pattern casting”, foam vaporization casting,
Styrocast, Foamcast, and Policast. The use of these terms has led to much confusion among design engineers, casting users, and casting producers.
The advantages of LFC include:
* Flexibility of foam: Foam is easy to manipulate, carve and glue, due to its unique properties.
* Dimensional accuracy: The patterns are accurate representations of the desired casting, as compared to
sand castingand there is no tool wear. There is also less finishing work required for an LFC casting, as there are no fins or parting lines.
* Elimination of cores: This allows for more complex casting designs, well-controlled wall thickness of castings, and no core-prints. This process also eliminates fins or shifts, core defects and sand mixing.
* Elimination of parting line: There is no draft and multiple levels of casting are possible. Proper gating and riser placement can be achieved, and there are no shifts or fins. Forms that are not typically possible with traditional
cope and dragmethods can be produced since the mold does not need to be parted to remove a pattern.
* Part consolidation: The flexibility of LFC often allows for consolidating the parts into one integral component; other forming processes would require the production of one or more parts to be assembled.
* Lower cost: Because the process is much simpler, as compared to traditional sand-casting methods, production cost is much lower.
Public recognition of the benefits of LFC was made by General Motors in
1993. By 1998, LFC production had reached approximately 140,00 tons in the United States alone. And in 2005, it is forecast that LFC will account for 29% of the aluminum, and 14% of the ferrous casting markets. 
Common metals cast
Commonly used metals include:
* ductile (or nodular) iron
copper-based casting alloys
Hot-wire foam cutter
Wikimedia Foundation. 2010.
Look at other dictionaries:
Lost foam casting — Lost foam casting. См. Литье с расходуемой моделью. (Источник: «Металлы и сплавы. Справочник.» Под редакцией Ю.П. Солнцева; НПО Профессионал , НПО Мир и семья ; Санкт Петербург, 2003 г.) … Словарь металлургических терминов
lost-foam casting — A casting method using foamed plastic cores, giving the surface of the castings the appearance of styrofoam; used for engine blocks … Dictionary of automotive terms
lost-foam casting process — A casting method using foamed plastic cores, giving the surface of the castings the appearance of styrofoam; used for engine blocks … Dictionary of automotive terms
Lost-wax casting — A model of an apple in wax … Wikipedia
Casting (metalworking) — Casting iron in a sand mold In metalworking, casting involves pouring liquid metal into a mold, which contains a hollow cavity of the desired shape, and then allowing it to cool and solidify. The solidified part is also known as a casting, which… … Wikipedia
casting —  A process technology that delivers a liquid molten metal into a purpose built mold. After cooling, the solid metal surface has the shape of the mold cavity.  Pouring metal into a mold to form an object. Also see die casting lost foam… … Dictionary of automotive terms
casting process — See lost foam casting process … Dictionary of automotive terms
Casting defect — A casting defect is an irregularity in the metal casting process that is undesired. Some defects can be tolerated while others can be repaired otherwise they must be eliminated. They are broken down into five main categories: gas porosity,… … Wikipedia
Full-mold casting — (similar to lost foam casting) is a process in which a polystyrene foam pattern is made and coated with a Refractory material. This foam pattern is then put into a one piece sand mold. After the hot metal is poured into the mold the foam… … Wikipedia
Investment casting — For investment casting in art, see lost wax casting. Investment casting, also called lost wax casting, is one of the oldest known metal forming techniques. From 5,000 years ago, when beeswax formed the pattern, to today’s high technology waxes,… … Wikipedia